#------------------------------------------------------------------------------
#$Date: 2016-02-14 16:26:36 +0200 (Sun, 14 Feb 2016) $
#$Revision: 176435 $
#$URL: svn://www.crystallography.net/cod/cif/2/20/72/2207204.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/. The original data for this entry
# were provided by IUCr Journals, http://journals.iucr.org/.
#
# The file may be used within the scientific community so long as
# proper attribution is given to the journal article from which the
# data were obtained.
#
data_2207204
loop_
_publ_author_name
'Ben Amor, Rym'
'Zid, Mohamed Faouzi'
_publ_section_title
;
NaCa~1.5~(NbO)₂O₂(AsO₄)₂
;
_journal_coeditor_code           DN6243
_journal_issue                   11
_journal_name_full               'Acta Crystallographica, Section E'
_journal_page_first              i228
_journal_page_last               i230
_journal_paper_doi               10.1107/S1600536805031429
_journal_volume                  61
_journal_year                    2005
_chemical_formula_iupac          'Na Ca1.5 (NbO)2 O2 (As O4)2'
_chemical_formula_moiety         'As Nb O6, 0.435(Ca), 0.315(Ca), 0.5(Na)'
_chemical_formula_structural     'Na Ca1.5 (NbO)2 O2 (As O4)2'
_chemical_formula_sum            'As2 Ca1.5 Na Nb2 O12'
_chemical_formula_weight         610.78
_chemical_name_systematic
;
sodium calcium niobate oxide arsenate
;
_space_group_IT_number           15
_symmetry_cell_setting           monoclinic
_symmetry_space_group_name_Hall  '-C 2yc'
_symmetry_space_group_name_H-M   'C 1 2/c 1'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                90.00
_cell_angle_beta                 113.8270(10)
_cell_angle_gamma                90.00
_cell_formula_units_Z            4
_cell_length_a                   6.730(2)
_cell_length_b                   22.302(3)
_cell_length_c                   7.4309(9)
_cell_measurement_reflns_used    25
_cell_measurement_temperature    298(2)
_cell_measurement_theta_max      14
_cell_measurement_theta_min      12
_cell_volume                     1020.3(4)
_computing_cell_refinement       'CAD-4 EXPRESS'
_computing_data_collection
;
CAD-4 EXPRESS (Duisenberg, 1992; Macíček & Yordanov, 1992;
Enraf--Nonius, 1994)
;
_computing_data_reduction        'XCAD4 (Harms & Wocadlo, 1995)'
_computing_molecular_graphics
;
DIAMOND (Brandenburg, 1998), ORTEPIII (Burnett & Johnson, 1996) and
ORTEP-3 for Windows (Farrugia, 1997)
;
_computing_publication_material  SHELXL97
_computing_structure_refinement  'SHELXL97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXS97 (Sheldrick, 1997)'
_diffrn_ambient_temperature      298(2)
_diffrn_measured_fraction_theta_full 0.999
_diffrn_measured_fraction_theta_max 0.999
_diffrn_measurement_device_type  'Enraf--Nonius CAD-4'
_diffrn_measurement_method       ω/2θ
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0152
_diffrn_reflns_av_sigmaI/netI    0.0250
_diffrn_reflns_limit_h_max       9
_diffrn_reflns_limit_h_min       -8
_diffrn_reflns_limit_k_max       31
_diffrn_reflns_limit_k_min       -1
_diffrn_reflns_limit_l_max       1
_diffrn_reflns_limit_l_min       -10
_diffrn_reflns_number            1683
_diffrn_reflns_theta_full        29.96
_diffrn_reflns_theta_max         29.96
_diffrn_reflns_theta_min         3.43
_diffrn_standards_decay_%        1.2
_diffrn_standards_interval_time  120
_diffrn_standards_number         2
_exptl_absorpt_coefficient_mu    9.544
_exptl_absorpt_correction_T_max  0.3857
_exptl_absorpt_correction_T_min  0.2605
_exptl_absorpt_correction_type   psi-scan
_exptl_absorpt_process_details   '(North et al., 1968)'
_exptl_crystal_colour            colorless
_exptl_crystal_density_diffrn    3.977
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       prisme
_exptl_crystal_F_000             1140
_exptl_crystal_size_max          0.16
_exptl_crystal_size_mid          0.12
_exptl_crystal_size_min          0.10
_refine_diff_density_max         0.653
_refine_diff_density_min         -0.745
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.101
_refine_ls_hydrogen_treatment    undef
_refine_ls_matrix_type           full
_refine_ls_number_parameters     91
_refine_ls_number_reflns         1495
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.101
_refine_ls_R_factor_all          0.0245
_refine_ls_R_factor_gt           0.0194
_refine_ls_shift/su_max          0.021
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w = 1/[σ²(Fo²)+(0.0195P)²+2.343P] where P = (Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0500
_refine_ls_wR_factor_ref         0.0514
_reflns_number_gt                1337
_reflns_number_total             1495
_reflns_threshold_expression     I>2σ(I)
_cod_data_source_file            dn6243.cif
_cod_original_sg_symbol_H-M      'C 2/c'
_cod_original_formula_sum        'As2 Ca1.5 Na1 Nb2 O12'
_cod_database_code               2207204
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-x, y, -z+1/2'
'x+1/2, y+1/2, z'
'-x+1/2, y+1/2, -z+1/2'
'-x, -y, -z'
'x, -y, z-1/2'
'-x+1/2, -y+1/2, -z'
'x+1/2, -y+1/2, z-1/2'
loop_
_atom_site_label
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_calc_flag
_atom_site_refinement_flags
_atom_site_occupancy
_atom_site_type_symbol
Nb 0.00565(4) 0.357919(10) 0.51029(3) 0.00618(8) Uani d . 1 Nb
As1 -0.5000 0.417962(18) 0.2500 0.00927(10) Uani d S 1 As
As2 0.0000 0.221982(17) 0.2500 0.00575(9) Uani d S 1 As
Na 0.5000 0.44084(10) 0.7500 0.0347(6) Uani d S 1 Na
Ca1 0.0000 0.48192(4) 0.2500 0.00806(16) Uani d SP 0.87 Ca
Ca2 -0.5000 0.27733(7) 0.2500 0.0219(3) Uani d SP 0.63 Ca
O1 -0.0977(3) 0.26328(9) 0.3858(3) 0.0134(4) Uani d . 1 O
O2 0.0000 0.32411(13) 0.7500 0.0086(5) Uani d S 1 O
O3 0.0752(4) 0.43450(10) 0.5814(3) 0.0132(4) Uani d . 1 O
O4 -0.3221(3) 0.36857(10) 0.4147(3) 0.0122(4) Uani d . 1 O
O5 0.3118(3) 0.32501(11) 0.5945(3) 0.0179(5) Uani d . 1 O
O6 -0.6303(4) 0.45972(11) 0.3518(4) 0.0212(5) Uani d . 1 O
O7 0.0000 0.37148(13) 0.2500 0.0092(5) Uani d S 1 O
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
As As 0.0499 2.0058 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Na Na 0.0362 0.0249 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Nb Nb -2.0727 0.6215 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Ca Ca 0.2262 0.3064 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_diffrn_standard_refln_index_h
_diffrn_standard_refln_index_k
_diffrn_standard_refln_index_l
-4 0 4
1 7 -4
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle
O3 Nb O7 . . 92.45(11)
O3 Nb O2 . . 101.45(10)
O7 Nb O2 . . 166.04(12)
O3 Nb O5 . . 98.13(10)
O7 Nb O5 . . 88.43(7)
O2 Nb O5 . . 88.30(7)
O3 Nb O4 . . 96.24(9)
O7 Nb O4 . . 92.97(6)
O2 Nb O4 . . 86.88(6)
O5 Nb O4 . . 165.49(9)
O3 Nb O1 . . 174.00(9)
O7 Nb O1 . . 82.02(10)
O2 Nb O1 . . 84.15(9)
O5 Nb O1 . . 84.07(9)
O4 Nb O1 . . 81.82(8)
O3 Nb Ca1 . . 47.76(7)
O7 Nb Ca1 . . 46.28(9)
O2 Nb Ca1 . . 147.48(8)
O5 Nb Ca1 . . 104.38(6)
O4 Nb Ca1 . . 86.83(6)
O1 Nb Ca1 . . 126.32(6)
O3 Nb Ca2 . 7_456 136.38(7)
O7 Nb Ca2 . 7_456 129.72(9)
O2 Nb Ca2 . 7_456 36.45(8)
O5 Nb Ca2 . 7_456 75.58(6)
O4 Nb Ca2 . 7_456 92.57(6)
O1 Nb Ca2 . 7_456 49.56(6)
Ca1 Nb Ca2 . 7_456 175.859(16)
O7 Nb Na . . 93.17(5)
O2 Nb Na . . 95.87(4)
O5 Nb Na . . 53.99(8)
O4 Nb Na . . 140.20(7)
O1 Nb Na . . 137.98(6)
Ca1 Nb Na . . 69.80(3)
Ca2 Nb Na 7_456 . 112.88(3)
O3 Nb Ca2 . . 134.75(7)
O7 Nb Ca2 . . 84.82(5)
O2 Nb Ca2 . . 86.29(4)
O5 Nb Ca2 . . 126.83(8)
O4 Nb Ca2 . . 39.16(7)
O1 Nb Ca2 . . 42.76(6)
Ca1 Nb Ca2 . . 108.023(19)
Ca2 Nb Ca2 7_456 . 69.254(14)
Na Nb Ca2 . . 177.76(2)
O6 As1 O6 . 2_455 111.60(18)
O6 As1 O4 . 2_455 109.89(11)
O6 As1 O4 2_455 2_455 112.30(12)
O6 As1 O4 . . 112.30(12)
O6 As1 O4 2_455 . 109.89(11)
O4 As1 O4 2_455 . 100.39(15)
O6 As1 Ca2 . . 124.20(9)
O6 As1 Ca2 2_455 . 124.20(9)
O4 As1 Na 2_455 5_566 129.80(7)
O4 As1 Na . 5_566 129.80(7)
Ca2 As1 Na . 5_566 180.0
O6 As1 Ca1 . . 115.97(9)
O4 As1 Ca1 2_455 . 128.74(7)
O4 As1 Ca1 . . 82.75(7)
Ca2 As1 Ca1 . . 112.972(16)
Na As1 Ca1 5_566 . 67.028(16)
O6 As1 Ca1 2_455 1_455 115.97(9)
O4 As1 Ca1 2_455 1_455 82.75(7)
O4 As1 Ca1 . 1_455 128.74(7)
Ca2 As1 Ca1 . 1_455 112.972(16)
Na As1 Ca1 5_566 1_455 67.028(16)
Ca1 As1 Ca1 . 1_455 134.06(3)
O1 As2 O1 . 2 113.67(14)
O1 As2 O5 . 8_455 112.50(11)
O1 As2 O5 2 8_455 107.22(11)
O1 As2 O5 . 7_556 107.22(11)
O1 As2 O5 2 7_556 112.50(10)
O5 As2 O5 8_455 7_556 103.32(18)
O1 As2 Ca2 . 1_655 113.93(8)
O5 As2 Ca2 8_455 1_655 131.15(7)
O5 As2 Ca2 7_556 1_655 76.66(8)
O1 As2 Ca2 2 . 113.93(8)
O5 As2 Ca2 8_455 . 76.66(8)
O5 As2 Ca2 7_556 . 131.15(7)
Ca2 As2 Ca2 1_655 . 139.71(5)
O6 Na O6 6_666 5_566 63.43(11)
O6 Na O3 6_666 . 75.81(8)
O6 Na O3 5_566 . 109.70(9)
O6 Na O3 6_666 2_656 109.70(9)
O6 Na O3 5_566 2_656 75.81(8)
O3 Na O3 . 2_656 173.81(14)
O6 Na O6 6_666 2_556 63.71(9)
O6 Na O6 5_566 2_556 100.55(8)
O3 Na O6 . 2_556 109.51(7)
O3 Na O6 2_656 2_556 71.49(7)
O6 Na O6 6_666 1_655 100.55(8)
O6 Na O6 5_566 1_655 63.71(9)
O3 Na O6 . 1_655 71.49(7)
O3 Na O6 2_656 1_655 109.51(7)
O6 Na O6 2_556 1_655 162.44(13)
O6 Na O5 6_666 . 136.76(7)
O6 Na O5 5_566 . 141.74(7)
O3 Na O5 . . 62.96(7)
O3 Na O5 2_656 . 111.00(9)
O6 Na O5 2_556 . 117.47(9)
O6 Na O5 1_655 . 79.07(7)
O6 Na O5 6_666 2_656 141.74(7)
O6 Na O5 5_566 2_656 136.76(7)
O3 Na O5 . 2_656 111.00(9)
O3 Na O5 2_656 2_656 62.96(7)
O6 Na O5 2_556 2_656 79.07(7)
O6 Na O5 1_655 2_656 117.47(9)
O5 Na O5 . 2_656 54.32(9)
O6 Na As1 6_666 5_566 31.71(6)
O6 Na As1 5_566 5_566 31.71(6)
O3 Na As1 . 5_566 93.10(7)
O3 Na As1 2_656 5_566 93.10(7)
O6 Na As1 2_556 5_566 81.22(7)
O6 Na As1 1_655 5_566 81.22(7)
O5 Na As1 . 5_566 152.84(5)
O5 Na As1 2_656 5_566 152.84(5)
O6 Na Nb 6_666 . 103.26(5)
O6 Na Nb 5_566 . 130.36(6)
O3 Na Nb . . 28.50(5)
O3 Na Nb 2_656 . 145.40(9)
O6 Na Nb 2_556 . 116.14(5)
O6 Na Nb 1_655 . 73.55(5)
O5 Na Nb 2_656 . 84.66(7)
As1 Na Nb 5_566 . 121.03(3)
O6 Na Nb 6_666 2_656 130.36(6)
O6 Na Nb 5_566 2_656 103.26(5)
O3 Na Nb . 2_656 145.40(9)
O3 Na Nb 2_656 2_656 28.50(5)
O6 Na Nb 2_556 2_656 73.55(5)
O6 Na Nb 1_655 2_656 116.14(5)
O5 Na Nb . 2_656 84.66(7)
O5 Na Nb 2_656 2_656 34.50(4)
As1 Na Nb 5_566 2_656 121.03(3)
Nb Na Nb . 2_656 117.95(6)
O6 Na Ca1 6_666 5_666 90.93(7)
O6 Na Ca1 5_566 5_666 37.68(5)
O3 Na Ca1 . 5_666 145.45(7)
O3 Na Ca1 2_656 5_666 39.25(5)
O6 Na Ca1 2_556 5_666 91.90(5)
O6 Na Ca1 1_655 5_666 80.08(5)
O5 Na Ca1 . 5_666 130.59(6)
O5 Na Ca1 2_656 5_666 99.22(5)
As1 Na Ca1 5_566 5_666 62.89(3)
Nb Na Ca1 . 5_666 151.852(12)
Nb Na Ca1 2_656 5_666 65.67(2)
O6 Ca1 O6 2_455 1_655 155.60(13)
O6 Ca1 O3 2_455 5_566 84.99(9)
O6 Ca1 O3 1_655 5_566 114.47(8)
O6 Ca1 O3 2_455 6_565 114.47(8)
O6 Ca1 O3 1_655 6_565 84.99(9)
O3 Ca1 O3 5_566 6_565 78.74(10)
O6 Ca1 O7 2_455 . 77.80(6)
O6 Ca1 O7 1_655 . 77.80(6)
O3 Ca1 O7 5_566 . 140.63(5)
O3 Ca1 O7 6_565 . 140.63(5)
O6 Ca1 O3 2_455 2 80.14(8)
O6 Ca1 O3 1_655 2 89.71(8)
O3 Ca1 O3 5_566 2 145.65(8)
O3 Ca1 O3 6_565 2 79.59(8)
O7 Ca1 O3 . 2 65.35(5)
O6 Ca1 O3 2_455 . 89.71(8)
O6 Ca1 O3 1_655 . 80.14(8)
O3 Ca1 O3 5_566 . 79.59(8)
O3 Ca1 O3 6_565 . 145.65(8)
O7 Ca1 O3 . . 65.35(5)
O3 Ca1 O3 2 . 130.70(10)
O6 Ca1 Nb 2_455 2 82.92(7)
O6 Ca1 Nb 1_655 2 77.05(6)
O3 Ca1 Nb 5_566 2 167.89(5)
O3 Ca1 Nb 6_565 2 107.01(5)
O7 Ca1 Nb . 2 34.759(11)
O3 Ca1 Nb 2 2 31.56(5)
O3 Ca1 Nb . 2 99.60(6)
O6 Ca1 Nb 2_455 . 77.05(6)
O6 Ca1 Nb 1_655 . 82.92(7)
O3 Ca1 Nb 5_566 . 107.01(5)
O3 Ca1 Nb 6_565 . 167.89(5)
O7 Ca1 Nb . . 34.759(11)
O3 Ca1 Nb 2 . 99.60(6)
O3 Ca1 Nb . . 31.56(5)
Nb Ca1 Nb 2 . 69.52(2)
O6 Ca1 As1 2_455 . 19.90(6)
O6 Ca1 As1 1_655 . 140.83(7)
O3 Ca1 As1 5_566 . 85.13(5)
O3 Ca1 As1 6_565 . 133.50(5)
O7 Ca1 As1 . . 67.028(16)
O3 Ca1 As1 2 . 90.83(5)
O3 Ca1 As1 . . 70.12(5)
Nb Ca1 As1 2 . 83.262(18)
Nb Ca1 As1 . . 58.402(12)
O6 Ca1 As1 2_455 1_655 140.83(7)
O6 Ca1 As1 1_655 1_655 19.90(6)
O3 Ca1 As1 5_566 1_655 133.50(5)
O3 Ca1 As1 6_565 1_655 85.13(5)
O7 Ca1 As1 . 1_655 67.028(16)
O3 Ca1 As1 2 1_655 70.12(5)
O3 Ca1 As1 . 1_655 90.83(5)
Nb Ca1 As1 2 1_655 58.402(12)
Nb Ca1 As1 . 1_655 83.262(18)
As1 Ca1 As1 . 1_655 134.06(3)
O6 Ca1 Na 2_455 5_666 157.77(6)
O6 Ca1 Na 1_655 5_666 42.86(7)
O3 Ca1 Na 5_566 5_666 91.23(6)
O3 Ca1 Na 6_565 5_666 43.44(6)
O7 Ca1 Na . 5_666 117.11(3)
O3 Ca1 Na 2 5_666 91.07(5)
O3 Ca1 Na . 5_666 111.19(5)
Nb Ca1 Na 2 5_666 100.24(3)
Nb Ca1 Na . 5_666 124.81(3)
As1 Ca1 Na . 5_666 175.86(4)
As1 Ca1 Na 1_655 5_666 50.08(3)
O2 Ca2 O4 7_456 . 146.99(5)
O2 Ca2 O4 7_456 2_455 146.99(5)
O4 Ca2 O4 . 2_455 66.03(10)
O2 Ca2 O1 7_456 2_455 82.79(6)
O4 Ca2 O1 . 2_455 122.85(8)
O4 Ca2 O1 2_455 2_455 70.61(7)
O2 Ca2 O1 7_456 . 82.79(6)
O4 Ca2 O1 . . 70.61(7)
O4 Ca2 O1 2_455 . 122.85(8)
O1 Ca2 O1 2_455 . 165.59(12)
O2 Ca2 O1 7_456 8_455 70.19(5)
O4 Ca2 O1 . 8_455 131.65(8)
O4 Ca2 O1 2_455 8_455 84.49(7)
O1 Ca2 O1 2_455 8_455 76.43(7)
O1 Ca2 O1 . 8_455 98.61(7)
O2 Ca2 O1 7_456 7_456 70.19(5)
O4 Ca2 O1 . 7_456 84.49(7)
O4 Ca2 O1 2_455 7_456 131.65(8)
O1 Ca2 O1 2_455 7_456 98.61(7)
O1 Ca2 O1 . 7_456 76.43(7)
O1 Ca2 O1 8_455 7_456 140.37(11)
O2 Ca2 As1 7_456 . 180.0
O4 Ca2 As1 . . 33.01(5)
O4 Ca2 As1 2_455 . 33.01(5)
O1 Ca2 As1 2_455 . 97.21(6)
O1 Ca2 As1 . . 97.21(6)
O1 Ca2 As1 8_455 . 109.81(5)
O1 Ca2 As1 7_456 . 109.81(5)
O2 Ca2 Nb 7_456 8_455 30.784(14)
O4 Ca2 Nb . 8_455 150.70(5)
O4 Ca2 Nb 2_455 8_455 124.66(5)
O1 Ca2 Nb 2_455 8_455 85.38(6)
O1 Ca2 Nb . 8_455 82.24(5)
O1 Ca2 Nb 8_455 8_455 40.85(5)
O1 Ca2 Nb 7_456 8_455 100.02(6)
As1 Ca2 Nb . 8_455 149.216(14)
O2 Ca2 Nb 7_456 7_456 30.784(14)
O4 Ca2 Nb . 7_456 124.66(5)
O4 Ca2 Nb 2_455 7_456 150.70(5)
O1 Ca2 Nb 2_455 7_456 82.24(5)
O1 Ca2 Nb . 7_456 85.38(6)
O1 Ca2 Nb 8_455 7_456 100.02(6)
O1 Ca2 Nb 7_456 7_456 40.85(5)
As1 Ca2 Nb . 7_456 149.216(14)
Nb Ca2 Nb 8_455 7_456 61.57(3)
O2 Ca2 As2 7_456 1_455 69.86(2)
O4 Ca2 As2 . 1_455 124.10(5)
O4 Ca2 As2 2_455 1_455 90.97(5)
O1 Ca2 As2 2_455 1_455 24.82(5)
O1 Ca2 As2 . 1_455 145.21(7)
O1 Ca2 As2 8_455 1_455 92.08(5)
O1 Ca2 As2 7_456 1_455 74.34(5)
As1 Ca2 As2 . 1_455 110.14(2)
Nb Ca2 As2 8_455 1_455 84.65(3)
Nb Ca2 As2 7_456 1_455 60.102(18)
O2 Ca2 As2 7_456 . 69.86(2)
O4 Ca2 As2 . . 90.97(5)
O4 Ca2 As2 2_455 . 124.10(5)
O1 Ca2 As2 2_455 . 145.21(7)
O1 Ca2 As2 . . 24.82(5)
O1 Ca2 As2 8_455 . 74.34(5)
O1 Ca2 As2 7_456 . 92.08(5)
As1 Ca2 As2 . . 110.14(2)
Nb Ca2 As2 8_455 . 60.102(18)
Nb Ca2 As2 7_456 . 84.65(3)
As2 Ca2 As2 1_455 . 139.71(5)
As2 O1 Nb . . 128.03(11)
As2 O1 Ca2 . . 116.65(11)
Nb O1 Ca2 . . 98.62(8)
As2 O1 Ca2 . 7_456 115.19(11)
Nb O1 Ca2 . 7_456 89.59(8)
Ca2 O1 Ca2 . 7_456 103.57(7)
Nb O2 Nb 2_556 . 134.47(16)
Nb O2 Ca2 2_556 7_456 112.77(8)
Nb O2 Ca2 . 7_456 112.77(8)
Nb O3 Ca1 . 5_566 143.58(11)
Nb O3 Ca1 . . 100.68(9)
Ca1 O3 Ca1 5_566 . 100.41(8)
Nb O3 Na . . 107.27(11)
Ca1 O3 Na 5_566 . 97.31(8)
Ca1 O3 Na . . 101.13(8)
As1 O4 Nb . . 131.75(12)
As1 O4 Ca2 . . 96.79(9)
Nb O4 Ca2 . . 108.77(9)
As2 O5 Nb 7_556 . 145.18(13)
As2 O5 Na 7_556 . 101.18(11)
Nb O5 Na . . 91.51(9)
As1 O6 Ca1 . 1_455 131.33(13)
As1 O6 Na . 5_566 92.49(11)
Ca1 O6 Na 1_455 5_566 99.46(9)
As1 O6 Na . 1_455 113.99(12)
Ca1 O6 Na 1_455 1_455 102.40(9)
Na O6 Na 5_566 1_455 116.29(9)
Nb O7 Nb 2 . 162.08(17)
Nb O7 Ca1 2 . 98.96(9)
Nb O7 Ca1 . . 98.96(9)
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_site_symmetry_2
_geom_bond_distance
Nb O3 . 1.793(2)
Nb O7 . 1.9428(6)
Nb O2 . 1.9488(12)
Nb O5 . 2.033(2)
Nb O4 . 2.040(2)
Nb O1 . 2.297(2)
Nb Ca1 . 3.3661(8)
Nb Ca2 7_456 3.5111(13)
Nb Na . 3.5880(14)
Nb Ca2 . 3.6378(11)
As1 O6 . 1.657(2)
As1 O6 2_455 1.657(2)
As1 O4 2_455 1.721(2)
As1 O4 . 1.721(2)
As1 Ca2 . 3.1363(16)
As1 Na 5_566 3.149(2)
As1 Ca1 . 3.6548(10)
As1 Ca1 1_455 3.6548(10)
As2 O1 . 1.684(2)
As2 O1 2 1.684(2)
As2 O5 8_455 1.690(2)
As2 O5 7_556 1.690(2)
As2 Ca2 1_655 3.5843(11)
As2 Ca2 . 3.5843(11)
Na O6 6_666 2.607(3)
Na O6 5_566 2.607(3)
Na O3 . 2.621(2)
Na O3 2_656 2.621(2)
Na O6 2_556 2.758(3)
Na O6 1_655 2.758(3)
Na O5 . 2.903(3)
Na O5 2_656 2.903(3)
Na As1 5_566 3.149(2)
Na Nb 2_656 3.5880(14)
Na Ca1 5_666 3.7802(14)
Ca1 O6 2_455 2.342(2)
Ca1 O6 1_655 2.342(2)
Ca1 O3 5_566 2.411(2)
Ca1 O3 6_565 2.411(2)
Ca1 O7 . 2.463(3)
Ca1 O3 2 2.536(2)
Ca1 O3 . 2.536(2)
Ca1 Nb 2 3.3661(8)
Ca1 As1 1_655 3.6548(10)
Ca1 Na 5_666 3.7802(14)
Ca2 O2 7_456 2.262(3)
Ca2 O4 . 2.426(3)
Ca2 O4 2_455 2.426(3)
Ca2 O1 2_455 2.498(2)
Ca2 O1 . 2.498(2)
Ca2 O1 8_455 2.672(2)
Ca2 O1 7_456 2.672(2)
Ca2 Nb 8_455 3.5111(13)
Ca2 Nb 7_456 3.5111(13)
Ca2 As2 1_455 3.5843(11)
O1 Ca2 7_456 2.672(2)
O2 Nb 2_556 1.9488(11)
O2 Ca2 7_456 2.262(3)
O3 Ca1 5_566 2.411(2)
O5 As2 7_556 1.690(2)
O6 Ca1 1_455 2.342(2)
O6 Na 5_566 2.607(3)
O6 Na 1_455 2.758(3)
O7 Nb 2 1.9428(6)
